DOI: 10.17188/1283394
title: Materials Data on RbAl3Cd(SiO4)3 by Materials Project

description: RbCdAl3(SiO4)3 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are four inequivalent Rb1+ sites. In the first Rb1+ site, Rb1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Rb–O bond distances ranging from 3.08–3.57 Å. In the second Rb1+ site, Rb1+ is bonded in a 3-coordinate geometry to four O2- atoms. There are a spread of Rb–O bond distances ranging from 2.79–3.59 Å. In the third Rb1+ site, Rb1+ is bonded in a 2-coordinate geometry to four O2- atoms. There are a spread of Rb–O bond distances ranging from 2.93–3.47 Å. In the fourth Rb1+ site, Rb1+ is bonded in a 3-coordinate geometry to two O2- atoms. There are one shorter (2.95 Å) and one longer (3.00 Å) Rb–O bond lengths. There are four inequivalent Cd2+ sites. In the first Cd2+ site, Cd2+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Cd–O bond distances ranging from 2.14–2.53 Å. In the second Cd2+ site, Cd2+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Cd–O bond distances ranging from 2.13–2.63 Å. In the third Cd2+ site, Cd2+ is bonded in a distorted rectangular see-saw-like geometry to four O2- atoms. There are a spread of Cd–O bond distances ranging from 2.13–2.40 Å. In the fourth Cd2+ site, Cd2+ is bonded in a trigonal non-coplanar geometry to three O2- atoms. There are one shorter (2.14 Å) and two longer (2.17 Å) Cd–O bond lengths. There are twelve inequivalent Al3+ sites. In the first Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.80 Å. In the second Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.75–1.77 Å. In the third Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.78 Å. In the fourth Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.79 Å. In the fifth Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.82 Å. In the sixth Al3+ site, Al3+ is bonded to four O2- atoms to form corner-sharing AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.71–1.81 Å. In the seventh Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.68–1.83 Å. In the eighth Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.68–1.84 Å. In the ninth Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.68–1.84 Å. In the tenth Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.68–1.80 Å. In the eleventh Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.72–1.80 Å. In the twelfth Al3+ site, Al3+ is bonded to four O2- atoms to form AlO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.74–1.81 Å. There are twelve inequivalent Si4+ sites. In the first Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.66 Å. In the second Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.62–1.67 Å. In the third Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.67 Å. In the fourth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.69 Å. In the fifth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.66 Å. In the sixth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.67 Å. In the seventh Si4+ site, Si4+ is bonded to four O2- atoms to form corner-sharing SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.64 Å. In the eighth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.68 Å. In the ninth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.65 Å. In the tenth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.62–1.64 Å. In the eleventh Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.65 Å. In the twelfth Si4+ site, Si4+ is bonded to four O2- atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.66 Å. There are forty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the second O2- site, O2- is bonded in a bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the third O2- site, O2- is bonded in a bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the fifth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the seventh O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the eighth O2- site, O2- is bonded in a linear geometry to two Si4+ atoms. In the ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one Al3+ and one Si4+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the eleventh O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the twelfth O2- site, O2- is bonded in a bent 150 degrees geometry to one Al3+ and one Si4+ atom. In the thirteenth O2- site, O2- is bonded in a linear geometry to one Al3+ and one Si4+ atom. In the fourteenth O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the fifteenth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Rb1+ and two Si4+ atoms. In the sixteenth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Rb1+ and two Si4+ atoms. In the seventeenth O2- site, O2- is bonded in a linear geometry to one Rb1+ and two Si4+ atoms. In the eighteenth O2- site, O2- is bonded in a linear geometry to two Si4+ atoms. In the nineteenth O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the twentieth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the twenty-first O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the twenty-second O2- site, O2- is bonded in a bent 150 degrees geometry to two Si4+ atoms. In the twenty-third O2- site, O2- is bonded in a bent 150 degrees geometry to one Al3+ and one Si4+ atom. In the twenty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one Al3+ and one Si4+ atom. In the twenty-fifth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Rb1+, one Al3+, and one Si4+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Al3+ and one Si4+ atom. In the twenty-seventh O2- site, O2- is bonded in a bent 150 degrees geometry to one Al3+ and one Si4+ atom. In the twenty-eighth O2- site, O2- is bonded in a 2-coordinate geometry to one Rb1+ and two Al3+ atoms. In the twenty-ninth O2- site, O2- is bonded in a 2-coordinate geometry to one Cd2+ and two Al3+ atoms. In the thirtieth O2- site, O2- is bonded in a 3-coordinate geometry to one Cd2+ and two Al3+ atoms. In the thirty-first O2- site, O2- is bonded in a 2-coordinate geometry to one Cd2+ and two Al3+ atoms. In the thirty-second O2- site, O2- is bonded in a 3-coordinate geometry to one Rb1+, one Cd2+, and two Al3+ atoms. In the thirty-third O2- site, O2- is bonded in a bent 150 degrees geometry to one Rb1+, one Cd2+, and two Al3+ atoms. In the thirty-fourth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Rb1+ and two Al3+ atoms. In the thirty-fifth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Cd2+ and two Al3+ atoms. In the thirty-sixth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Rb1+, one Cd2+, and two Al3+ atoms. In the thirty-seventh O2- site, O2- is bonded in a linear geometry to two Al3+ atoms. In the thirty-eighth O2- site, O2- is bonded in a linear geometry to two Al3+ atoms. In the thirty-ninth O2- site, O2- is bonded in a 3-coordinate geometry to one Cd2+, one Al3+, and one Si4+ atom. In the fortieth O2- site, O2- is bonded in a trigonal planar geometry to one Cd2+ and two Al3+ atoms. In the forty-first O2- site, O2- is bonded in a distorted trigonal planar geometry to one Cd2+, one Al3+, and one Si4+ atom. In the forty-second O2- site, O2- is bonded in a 3-coordinate geometry to one Cd2+, one Al3+, and one Si4+ atom. In the forty-third O2- site, O2- is bonded in a 3-coordinate geometry to one Cd2+, one Al3+, and one Si4+ atom. In the forty-fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Cd2+ and two Al3+ atoms. In the forty-fifth O2- site, O2- is bonded in a trigonal planar geometry to one Cd2+ and two Al3+ atoms. In the forty-sixth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Cd2+, one Al3+, and one Si4+ atom.